The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints


 Marcus Eustace Whitehead
 8 months ago
 Views:
Transcription
1 , June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed to investigate the choice of failure criterion based on characteristic length method for predicting composite joint strength. The available experimental data for joint strength in literature were used to determine the accuracy of analytically obtained results. The analysis utilized six failure criteria, where it was shown that among the failure criteria investigated no one gave a best fit for all the three plates evaluated for strength, and the fit of individual failure theories is variable from one type of material to another. The results also showed that the accuracy of this method can be improved by computing the average predicted values of more than three failure criteria. Index Terms Characteristic length, Composite, Failure Criteria, and Joint strength. I. INTRODUCTION Adhesive bonding and mechanical bonding remain the two most common methods of joint design. While an adhesive joint offers the advantage of distributing the load over a larger area than a mechanical joint, its use is very restrictive due to its sensitivity to environmental conditions such as temperature and humidity. Therefore, mechanical joints are widely used as a reliable and practical method to assemble the composite parts that constitute a mechanical structure; they offer the advantage of assembly and disassembly for accessibility and maintenance, and reliability at various environmental conditions. However, a significant drawback when using the mechanical joint is that it always requires joint holes, which can be a source of stress concentration and thereby weakens the intended strength for the structures. Therefore, for the design of composite joints, stress and failure analysis around the fastener hole should first be conducted. During the loading of mechanical joints, the laminate deforms as the applied load increases and the contact surface between the fastener and the plate changes. It should be noted that despite the fact that the distributed stress around the fastener hole could be accurately determined, the failure at any point within the stress concentration region does not necessarily lead to failure of the joints. The strength of the structure will be underestimated if local failure is taken to be the ultimate failure of the joint. It becomes a big task to develop an analytic or computational method that can Manuscript submitted March 2, The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints. Olanrewaju Aluko is with the University of MichiganFlint, 303 E. Kearsley Street, Flint, MI USA (phone: ; fax: ; umflint.edu). Quamrul Mazumder., is with University of MichiganFlint, 303 E. Kearsley Street, Flint, MI 48502, USA. ( adequately model the complicated failure and structural response to loading of composite joints. Because of the complexity of the failure of composite joints coupled with the intension to reduce the cost and materials wastage in practical testing to failure, the analytical determination of bolted joint strength has received the attention of many researchers [1][16]. One of the most common and efficient methods of predicting the strength is the characteristic length method. This method was proposed by Whiney and Nuismer [1][3], and it has been further developed by Chang et. al [4]. For this improved method, both the characteristic lengths in tension, R t, and compression, R c, must be determined by stress analysis associated with the results of bearing and tensile tests on notched and unnotched plates before employing an appropriate failure theory along the characteristic curve, r c as shown in Figure 1. By definition, the characteristic length (in tension or compression) is the radial distance from the hole boundary over which the plate must be critically stressed to initiate a sufficient flaw that can cause failure. Wang et al. [5] analytically determined failure strength of composite joints in both circular and elliptical holes using stress functions developed by Lehknitskii [6] and TsaiWu failure criterion. However, only characteristic length in tension was used around the hole boundary to evaluate the failure load and mode of the composite joint. Whitworth et al. [7], [8] utilized the characteristic curve developed by Chang et. al [4] (which requires both the characteristic length in tension and compression to be determined) along with Yamada failure criterion to evaluate joint strength. Kweon et al. [9] developed a new method for finding the characteristic length in terms of arbitrarily applied loads, as an alternative to the failure load of notched plate in tension and bearing load of the plate when in compression. They evaluated the joint strength along the characteristic curve using TsaiWu failure criterion. In spite of the significant effort that has been invested on strength estimation of composite joints by various investigators using characteristic length method, the choice of an effective failure criterion in order to improve the accuracy of the characteristic dimensions remains to be investigated. For this paper, various failure criteria were utilized with the characteristic length method to predict the strength of composite joints with the objective to optimize the prediction accuracy of the characteristic length method. A twodimensional analysis which utilized stress functions for the computation of stresses at the hole boundary and within the plate was employed. In this investigation of the effective choice of failure criterion on the prediction accuracy of joint strength, six selected failure criteria based on the previous survey by Nahas [10] were utilized.
2 , June 30  July 2, 2010, London, U.K. II. CHARACTERICTIC LENGTHS METHOD As stated earlier, one of the most common and efficient methods of predicting joint strength is the characteristic length method. This study utilized the characteristic curve first proposed by Chang et al. [4], which requires both the characteristics length in tension, R t and compression, R c. These must be determined by stress analysis associated with the results of nobearing and tensile tests on notched and unnotched plates before employing an appropriate failure theory along the characteristic curve, r c as shown in Fig. 1. This characteristic curve which can be (1) where x and y are equal to r c cos θ and r c sin θ respectively. In this study, the plate (MO1) made from carbonepoxy unidirectional prepreg (USN125) and plain weave prepreg (HPW193) [11] with stacking sequence [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] was used. The notation ±45 is used to represent a plane weave carbon/epoxy layer and the lamina thicknesses of the unidirectional and woven fabric layers are mm and 0.19 mm respectively. The hole diameter (d) is 9.53 mm, the width (W) of the plate is 26.8 mm, and the edge distance (e) is 19 mm. MO2 composite plate [9] was also utilized, having the same stacking sequence as above. The unidirectional layers are from the USN125 graphite/epoxy prepreg by Hankook Fiber Glass. The DMS2288 graphite/epoxy woven fabrics are by Sunkyong. The oneplythicknesses of the unidirectional and woven fabric layers are mm and mm, respectively. Other geometries of these two plates are the same. Additionally, AS4/ graphite/epoxy laminate having the stacking sequence [(45/0/45/0/90/0/45/0/45/0) 2 ] s with geometry of diameter (d), thickness (h), ratio of end distance to hole diameter (e/d) equal to cm, cm and 2, respectively was also used in this analysis [7]. The material properties of the three laminates are as given in Table I. a) Compressive characteristic length This analytical method employs the new approach proposed by Kweon et al. [9], without bearing tests to evaluate characteristic length in compression. This method utilizes any arbitrary load to compute the mean bearing stress, defined by: (2) where, P m, d and h are the arbitrary loads, diameter of hole and laminate thickness respectively. Within the context of this method, the compressive characteristic length R c as showed in Fig. 2 for point stress criterion [1] is the distance from the front holeedge to a point where the local compressive stress by the arbitrarily applied load is the same as the mean bearing stress. The present study utilized an analytical technique proposed by Aluko [12] to determine the compressive characteristic length. The analysis involved the stress functions that were computed from the displacement expressions that satisfy the boundary conditions. The semiinfinite plate in compression is as shown in Fig. 3. The boundary conditions of this geometry can be (3) (4) (5) where u and v are the displacements along x and y axes respectively. Therefore, the displacements u and v along the hole can be expressed by the following trigonometric series, (6) (7) where u 1, u 2, v 1 and v 2 are the unknowns to determine from boundary conditions. The condition of at free surface where x equal zero is: (8) Substituting (6) and (7) into (3), (4) and (5), we have Table I. The material properties of composite materials Propertie s Type of Material USN 125 HPW 193 DMS 2288 AS E 1 (GPa) E 2 (GPa) G 12 (GPa) υ X c (MPa) X t (MPa) Y c (MPa) Y t (MPa) S 12 (MPa) P m R c σ r =σ b d R t R c θ r c Characteristic curve Fig. 1. Schematic diagram for characteristic curve Fig. 2. Schematic diagram of the compressive characteristic length and normal stress distribution pattern
3 , June 30  July 2, 2010, London, U.K. θ y P Tensile stress distribution P R t Fig. 3. Schematic representation of compressive loading (9) The stress functions that satisfy the above displacement boundary conditions are [6]: (10) (11) However, the stresses in rectangular coordinate can be (12) Further, the stresses in polar coordinates can be obtained by stress transformations. In this model, frictionless condition is assumed between the pin and plate, Therefore, constant u o and c can be obtained from: (13) b) Tensile characteristic length x (14) Joints evaluation by the characteristic length method also requires the determination of tensile characteristic length. This involves the tensile test of notched (σ no) and unnotched (σ un ) laminate, as the strength values for the notched and unnotched laminates in tension must be known a priori. Fig. 4 shows the stress distribution of an infinite plate with a throughtothickness hole subjected to distributed tensile loads per unit area, P at infinity. The tensile stress would be highest at the side edges of the hole, and decreases further away from the side edges of the hole as shown in Fig. 4. In this analysis, the idea proposed by Konish and Whitney [13] for the approximate solution to the normal stress distribution σ y (x,0) in an infinite orthotropic plate with an open hole loaded in tension would be utilized. This solution can be (15) where the stress concentration factor K T and are expressed by the following: (16) (17) Tensile strength Fig. 4. Schematic diagram of the tensile characteristic length and stress distribution pattern where A ij, i,j = 1,2,6 denote the effective laminate inplane stiffness with 1 and 2 parallel and perpendicular to the loading direction respectively. The point stress criterion [2] can be applied to (15) to compute the tensile characteristic length at which failure analysis of the joint should be evaluated. The criterion defines the tensile characteristic length as the distance from the sideedge of the hole to a point where the tensile stress is the same as the strength of unnotched laminate. This can be (18) where, (19) The criterion assumes that the stress at infinity that determines the characteristic length defines the strength of the notched laminate. Substituting (17) and (18) into (15), the ratio of unnotched to notched strength is obtained as: (20) The value of tensile characteristic length can be determined if the data for tensile notched and unnotched laminate strength are known. The experimental values of notched and unnotched strength as obtained in the literature and the calculated values of both compressive and tensile characteristic length are shown in Table II. III. JOINT STRENGTH AND FAILURE ANALYSIS The present approach utilized an analytical technique that considers the orthotropic plate loaded with a force P by a rigid and frictionless pin (as shown in Fig. 5) to be homogeneous and infinite. In addition, the pin has the same diameter as the circular hole in the plate. Let the displacement of the plate due to pin load along x axis and at the ends of contact boundary be c o and c 1, respectively. Therefore, the boundary conditions of the geometry shown in Fig. 5 can be expressed as follows: (21) Table II: Characteristic length and strength data for the plates Plate R c, m R t, m Notched strength, MPa Unnotched strength, MPa MO MO AS
4 , June 30  July 2, 2010, London, U.K. (22) (23) where u and v are the displacements along x and y axes respectively. The condition for no contact surface can be (24) (25) Using (6) and (7) to satisfy the above displacement boundary conditions, we calculated the unknown u i and v i to be: (26a) (26b) The stress functions that satisfy the above displacement boundary conditions are [6]: (35) The prime implies the derivative of the stress functions. The parameters c o and c 1 can be determined from material properties of the plate and the condition of traction at the hole boundary. The traction for the case frictionless condition can be (36) (37) (27a) (38a) (27b) The stresses in rectangular coordinates can be expressed as [6]: (28a) (28b) (28c) where bar implies conjugate and (29) (30) (31) (32) (33) with a ij, i,j =1,2,6 are the compliances, and μ 1 and μ 2 are the roots of characteristics equation for orthotropic plate defined by: (34) where 1 and 2 are parallel and transverse to the loading direction, respectively, and r is the radius of the hole. The stresses in polar coordinates are given by the expressions: x Fig. 5. Schematic representation of composite joint P θ y (38b) Parameters k, n and g are materials constant of the plate (40) The stress results computed from above analytical method along the characteristic curve (shown in Fig. 1) were used in failure analysis to predict the joint strength for first ply failure. In an attempt to increase the accuracy of joint strength prediction by characteristic length method, six failure criteria based on the previous survey by Nahas [10] were used in conjunction with characteristic dimensions for the evaluation. In his survey, Nahas referenced the previous study by Burk [15] stating that AzziTsai and TsaiWu are among the four most commonly used failure criteria. Nahas also referenced the work of Owen and Rice [16] that asserts Fischer theory provides the best overall fit for static test results. The various failure criteria utilized in this analysis include the following [10]: YamadaSun: (41) AzziTsai: (42) Fisher: TsaiWu: (43) (44) Norris: (45) NorrisMckinnon: (46) Where σ 1 and σ 2 are longitudinal stresses and τ 12 is shear stress, X and Y are the ply longitudinal strength and S the ply shear strength. In this model, failure is expected to occur when the above equations are met. The computer code used to test for the condition of failure was written in Mathematica. The concept of finitewidth correction factor developed by Tan [14] was utilized to correct the infinite assumption of the plate. By definition, finitewidth correction factor (FWC) is a scale factor which is applied to multiply the notched infinite plate solution to obtain the notched
5 , June 30  July 2, 2010, London, U.K. finiteplate result based on the assumption that the normal stress profile for a finite plate is identical to that for an infinite except for a FWC factor. This correction factor is given by the relationship: (47) K T /K T is the FWC factor and K T and K T denote the stress concentration at the opening edge on the axis normal to the applied load for a finite plate and an infinite plate, respectively. The parameters σ N and are the failure strength of finitewidth and infinite plates, respectively. This factor is expressed by the relationship [14]: (48) where r is the radius of the hole and w defines the width of the plate. IV. RESULTS AND DISCUSSION The failure loads computed from the above analysis with failure criteria and their percentage differences with the experimentally obtained value for three different composite plates are shown in Table III. It can be seen from this table that no criterion provided the best fit for all the plate evaluated, and the fit of individual failure theories is variable from one type of material to another. Documented in Fig. 6 is the predicted load for MO1 plate as compared with experimental value. Due to variability in material properties, the experimental value for this plate [11] varies between 11.3 and 13.0 kn, which can be approximated to ±7.13% over the mean value. It can be depicted from this figure that all the predictions except TsaiWu which over estimated the strength are suitable for this plate. Keweon et al. [9] showed that seven specimens were tested for plate MO2 and the computed coefficient of variation (defined as standard deviation over the mean failure load) was equal to 6.1 percent. Even though the range for the experimental failure load cannot be computed from the coefficient of variation, it is evident from Fig. 7 that Fisher criterion is not an adequate predictor of strength. Therefore, the conclusion reached by Owen and Rice [16] that the Fisher theory provides the best overall fit for static tests results does not apply to all plates, as shown in this figure. Fisher theory severely underestimated the failure strength for MO2 plate. For AS plate, no information with regard to material variability was given. Notwithstanding, all the various criteria employed in this study appear to be adequate for the plate as documented in Fig. 8, with Fisher criterion yielding the best prediction. It should be noted that while TsaiWu failure theory over estimates the failure strength for all the three plates evaluated, the calculated average values of each prediction give a better fit for all the plates. V. CONCLUSION Stress analysis was performed to predict failure strength of pin loaded composite joints using the six failure criteria and on ChangScottSpringer characteristic curve model. The characteristic length in compression and tension that defines the characteristic curve was obtained by stress analysis associated with no bearing test and tensile test on laminate with and without a hole. The available experimental data in literature for different laminated composites were used to evaluate the joints strength. The agreement between Table III: Predicted loads and the percentage difference between experimental values Failure criteria MO1 (kn) MO2 ( kn) AS ( kn) MO1 (%) MO2 (%) AS (%) Experiment Yamada Sun AzziTs ai Norrs Mckinn on Norris Fisher TsaiW u Average Fig. 6: Failure predictions for MO1 Plate, [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] Fig.7: Failure predictions for MO2 plate, [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] experimental bearing strength for three different laminated composite plates evaluated and the analytically obtained joint strength by characteristic length method for each depends on the choice of failure criterion.
6 , June 30  July 2, 2010, London, U.K. Fig. 8: Failure predictions for AS Plate, [(45/0/45/0/90/0/45/0/45/0) 2 ] s There is no single failure criterion provided the best fit for all the plates evaluated; the average value of the predicted results from the six failure criteria investigated showed close agreement. Therefore, in order to optimize the accuracy of characteristic length method for joint strength prediction, three or more failure theories must be employed and an average calculated. REFERENCES [1] R.J. Nuismer, 1979, Application of the average stress failure criterion: Part II  Compression, Journal of composite materials, 13, pp [2] J.M. Whitney, and R.J. Nuismer, 1974, Stress fracture criteria for laminated composites containing stress concentrations, Journal of composite materials, 8 (253), pp [3] J.M. Whitney, and R.J. Nuismer, 1975, Uniaxial failure of composite laminated containing stress concentrations, Fracture mechanics of composite, ASTM STP, pp [4] F.K. Chang, and R.A. Scott, 1982, Strength of mechanically fastened composite joints, Journal of composite materials, 16, pp [5] J.T. Wang, C.G. Lotts, and D.D. Davis, Analysis of boltloaded elliptical holes in laminated composite joints. Journal of reinforced plastics and composites 1985;12: [6] Lekhnitskii, S.G., 1968, Anisotropic plates, Translated from the 2 nd Russian edition by S.W. Tsai, and T. Chevron, Gordon and Breach, London [7] H. A. Whitworth, M. Othieno, and O. Barton, 2003, Failure analysis of composite pin loaded joints, Composite structures, 59, pp [8] H. A. Whitworth, O. Aluko, and N.A. Tomlinson, 2008, Application of point stress criterion to the failure of composite pinned joints, Engineering fracture mechanics, 75, pp [9] J. Kweon, H. Ahn, and J. Choi, 2004, A new method to determine the characteristic lengths of composite joints without testing, Composite structures, 66, pp [10] M.N. Nahas, 1986, Survey of failure and postfailure theories of laminated fiberreinforced composites, Journal of composites technology and research, 8(4), pp [11] J. Choi, and Y. Chun, 2003, Failure load prediction of mechanically fastened composite joints, Journal of composite materials, 37(24), pp [12] O. Aluko, 2009, Analytic determination of compressive characteristic length of composite plate, Early career journal, ASME 8, pp [13] J.H. Konish, and J.M. Whitney, 1975, Approximate stresses in an orthotropic plate containing a circular hole, Journal of composite materials, 9, pp [14] S.C. Tan, 1988, Finitewidth correction factors for anisotropic plate containing a central opening, Journal of composite materials, 22, pp [15] R.C. Burk, 1983, Standard failure criteria needed for advanced composites, astronautics and aeronautics, 22, pp [16] M.J. Owen, and D.J. Rice, 1981, Biaxial strength behavior of glass fabricreinforced polyester resin, composites, 12, pp
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationMECHANICS OF MATERIALS
Fifth SI Edition CHTER 1 MECHNICS OF MTERILS Ferdinand. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Introduction Concept of Stress Lecture Notes: J. Walt Oler Teas Tech University Contents
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationSTRESS. Bar. ! Stress. ! Average Normal Stress in an Axially Loaded. ! Average Shear Stress. ! Allowable Stress. ! Design of Simple Connections
STRESS! Stress Evisdom! verage Normal Stress in an xially Loaded ar! verage Shear Stress! llowable Stress! Design of Simple onnections 1 Equilibrium of a Deformable ody ody Force w F R x w(s). D s y Support
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationInternational Conference on Mechanics and Civil Engineering (ICMCE 2014)
International Conference on Mechanics and Civil Engineering (ICMCE 2014) Parametric Design and Experimental Study for Weak Area Structure of Circle Composite Fragile Cover Ran CAO 1,a, GuangMing ZHOU
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationCRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES
S. Kakay et al. Int. J. Comp. Meth. and Exp. Meas. Vol. 5 No. (017) 116 14 CRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES SAMDAR KAKAY DANIEL BÅRDSEN
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationBolted Busbar Connections with Slotted Bolt Holes
Bolted Busbar Connections with Slotted Bolt Holes RAINA TZENEVA 1, YANKO SLAVTCHEV 2 and VALERI MLADENOV 3 1 Department of Electrical Apparatus, Faculty of Electrical Engineering, Technical University
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More information